Coked Ni/Al 2 O 3 from the catalytic reforming of volatiles from co-pyrolysis of lignin and polyethylene: preparation, identification and application as a potential adsorbent †

A novel and eco-friendly C – Ni/Al 2 O 3 composite was prepared through Ni/Al 2 O 3 coking during the catalytic reforming of volatiles from co-pyrolysis of lignin and polyethylene. The influence of Ni loading (0 – 20%) in the Ni/Al 2 O 3 catalyst and catalytic reforming temperature (500 – 800 ° C) on the characteristics of the C – Ni/ Al 2 O 3 composite was investigated, involving the analysis of SEM, XRD, TPO and FTIR. Fibrous carbon on the C – Ni/Al 2 O 3 composite was produced by the catalyst Ni(10%)/Al 2 O 3 at reforming temperatures of 600 and 700 ° C, which was oxidized at around 500 ° C according to the TPO analysis. The maximum deposition of carbon in the C – Ni(10%)/Al 2 O 3 composite was about 10.86%, achieved at a catalytic reforming temperature of 700 ° C. Abundant oxygen-containing functional groups were observed on the C – Ni/Al 2 O 3 composite through the FTIR analysis, leading to the outstanding adsorption performance for pollutant removal from aqueous systems. The optimal C – Ni/Al 2 O 3 composite was selected to investigate the effect of process conditions on the adsorption performance for Pb( II ), Cr( VI ), rhodamine B (RhB) and methyl orange (MO). The adsorption isotherms for the four mentioned pollutants were well fitted by the Langmuir model and the maximum adsorption amount for Pb( II ), Cr( VI ), RhB and MO was estimated to be 223.52, 54.90, 290.76 and 95.71 mg g − 1 , respectively. The results indicated that the as-prepared C – Ni/Al 2 O 3 composite had potential for the removal of heavy metal ions and hazardous organic compounds from aqueous systems.


Introduction
The utilization of lignin, which is the main residue in the papermaking industry, has been widely investigated in recent years, which not only can produce high-value chemicals or carbon materials, but also can reduce the impact of solid wastes on the environment. 1 Co-pyrolysis is considered as a promising technique for converting solid wastes into valueadded products, and adding a catalyst in the pyrolysis process can further enhance the conversion efficiency of feedstock and the yield of and selectivity to target products. [2][3][4][5] Catalysts can be mixed with raw materials directly, 6 or located under the raw material to catalyze the pyrolysis volatiles, 7 which have different influences on the formation of products. In addition, the effects of catalytic temperature, the ratio of feedstock to catalyst, the properties of the catalyst and other parameters on the distribution of products are important for catalytic co-pyrolysis of solid wastes. 8,9 Carbon materials, as one of the main products from the pyrolysis of solid wastes, are mainly produced at the temperature of 250-1000°C with a heating rate of about 5-50°C min −1 . 10 These carbon materials have high specific surface areas, abundant adsorption sites, good thermal stability, and controllable morphology, and exhibit huge potential as adsorbents for removing heavy metal ions, dyes and other pollutants in wastewater. 11,12 For example, biochar, one type of carbon material, produced from lignin-rich residues showed excellent adsorption capacities for heavy metal ions (Pb 2+ , Cu 2+ , Cd 2+ ) due to well-developed pore structures, high surface area and acid groups. 13 Li et al. also synthesized porous carbons by the co-pyrolysis of cyanobacteria and plastics, and applied the carbons for the treatment of wastewater containing methylene blue (MB); it was found that the as-synthesized carbon materials exhibited excellent adsorption of MB (maximum 490 mg g −1 ) because of the high surface area and pore volume. 3 However, pure carbon materials have low dispersion and strong hydrophobicity in aqueous solution, confining their application in the adsorption treatment of wastewater. 14 Carbon composites have been investigated to overcome the defects of pure carbon materials by modifying the carbon materials through oxidization, functional group grafting, and compositing with inorganic substances. 15,16 For example, Chen et al. found that carbon nanotube composites decorated with Ca/Al layered double hydroxide exhibited a high adsorption capacity for U(VI), and the maximum adsorption capacity for U(VI) onto these composites was four times higher than that onto bare carbon nanotubes. 17 In the study of Yari Moghaddam et al., a graphene oxide/almond shell composite fabricated by a freeze-drying method showed higher effectiveness than a pure graphene oxide in the removal of cadmium(II) and nickel(II). 18 Nevertheless, a complex synthesis process is often needed for the preparation of an ideal carbon composite, which produces many by-products and requires additional costs.
The catalysts used in the catalytic pyrolysis of solid wastes are easily coked with carbon that is composed of amorphous carbon and ordered graphite carbon, 19 which brings about catalyst deactivation. 20,21 Although studies on the regeneration of catalysts have been addressed in many reports, the catalytic performance of catalysts ultimately reduced due to repeated regeneration treatment, and even losing the catalytic activity. Arregi et al. carried out consecutive reaction-regeneration cycles of a Ni catalyst in the catalytic steam reforming of biomass pyrolysis volatiles, finding that the catalyst is only partially regenerated by coke combustion and the deactivation in each reaction step is faster as the number of successive cycles increased due to the irreversible deactivation caused by sintering of Ni species. 22 From another perspective, abundant oxygen-containing functional groups can be found in the deposited carbon on the catalyst with the migration of oxygen from the raw materials, such as biomass and lignin, which would bring new applications for the coked catalyst. Therefore, the used catalysts that have lost catalytic activity could be used for other applications.
The aim of this study is to explore the feasibility of the development of a carbon-catalyst composite and apply it as the adsorbent for the removal of heavy metal ions and dyes from aqueous solutions. The C-Ni/Al 2 O 3 composite was produced through carbon deposition on a Ni/Al 2 O 3 catalyst from catalytic reforming of volatiles derived from co-pyrolysis of lignin and polyethylene. SEM and TPO analyses were carried out to obtain the assembly patterns between the metal and deposited carbon, while XRD and FTIR analyses were adopted to identify the variation of metal distribution and surface functional groups of the composite against the metal loading and catalytic reforming temperature. The adsorption behavior of the composites was investigated by using Pb(II) and Cr(VI) as the model heavy metal ion pollutants and rhodamine B (RhB) and methyl orange (MO) as the model dye pollutants. The results of the adsorption experiments estimate the potential of the C-Ni/Al 2 O 3 composite as a commercial adsorbent for the removal of heavy metal ions and dyes from water systems.

Raw materials and chemicals
A lignin sample was extracted by using an acid precipitate method from a black liquor which was collected from a pulping company in Hunan Province, China. The detailed extraction process can be found in the literature. 23 Polyethylene powder with an average Mw and Mn of about ∼4000 and ∼1700 by GPC, respectively, was purchased from Sigma-Aldrich Corporation (St. Louis, MO, USA). The proximate analysis and ultimate analysis of the lignin sample and polyethylene are presented in the ESI † (Table S1) associated with this article. Nickel nitrate hexahydrate, alumina, lead nitrate, chromic nitrate nonahydrate, rhodamine B, methyl orange, nitric acid and sodium hydroxide used in this study were all analytical reagent grade and were purchased from Nanjing Zhongdong Huabo Instrument Co. LTD. Water used in preparing solutions was purified using an ultra-pure water system (Nanopure water, Barnstead).

Preparation of the C-Ni/Al 2 O 3 composite
The co-pyrolysis sample was pretreated according to the procedure described in the literature. 6 In brief, lignin was firstly impregnated in nickel nitrate solution, and then mixed with polyethylene powder after drying overnight. The concentration of metallic Ni in the co-pyrolysis sample was 1 mmol g −1 and the ratio of lignin and polyethylene was 1 : 1. The catalyst used in the catalytic reforming process was Ni/ Al 2 O 3 with different Ni loadings (5, 10, 20%) prepared by an impregnation method, and the as-prepared catalyst was denoted Ni(5%)/Al 2 O 3 , Ni(10%)/Al 2 O 3 , and Ni(20%)/Al 2 O 3 , respectively.
The catalytic reforming of the volatiles from co-pyrolysis of lignin and polyethylene was carried out in a two-stage vertical fixed bed reactor. At the beginning of the experiment, 2 g co-pyrolysis samples and 1 g Ni/Al 2 O 3 catalyst were added in the first stage (pyrolysis zone) and second stage (catalytic reforming zone), respectively. Then, high purity nitrogen was injected into the reactor with a flow rate of 100 mL min −1 to remove air. After injecting for 20 min, the second stage was first heated to the set-point temperature with a heating rate of 40°C min −1 , and then the first stage was heated to 800°C at a heating rate of 10°C min −1 . The residence time for the

Characterization of the C-Ni/Al 2 O 3 composite
The morphological characteristics of the as-synthesized C-Ni/ Al 2 O 3 composite were observed by scanning electron microscopy (SEM) (Inspect F50, FEI, USA). X-ray diffraction (XRD) patterns of the C-Ni/Al 2 O 3 composite were obtained using a Smartlab XRD-3 with Kα radiation and the scans were taken at the 5-80°2θ range. Raman spectra were determined by using a confocal LabRAM HR Evolution Raman spectroscopic system (HORIBA Scientific) with a 532 nm laser. The pyrolysis behavior and thermal stability of these C-Ni/Al 2 O 3 composites were analyzed through temperature programmed oxidation (TPO) on a thermogravimetric analyzer (TG209 F3, Netzsch, German). About 10 mg of the C-Ni/Al 2 O 3 composite was heated to 800°C under 100 mL min −1 air flow at a heating rate of 10°C min −1 and kept for 10 min. The functional group change of the C-Ni/Al 2 O 3 composite under different conditions was qualitatively studied using a Fourier transform infrared spectroscopy (FTIR) analyzer (Nicolet 6700, Thermo Fisher Scientific, USA) with the wavenumber range of 600-4000 cm −1 . The N 2 adsorption/desorption isotherms of the synthesized C-Ni/ Al 2 O 3 composites were investigated by using nitrogen adsorption measurement at 77 K (Quantachrome IQ3, USA). The specific surface areas were calculated through the Brunauer-Emmett-Teller (BET) method, while the pore size distributions of the composites were obtained from the analysis of the desorption values by using the Barrett-Joyner-Halenda (BJH) method.

Adsorption of heavy metal ions and dyes with the C-Ni/ Al 2 O 3 composite
Pb(II), Cr(VI), RhB and MO were chosen as model pollutants to investigate the adsorption performance of the C-Ni/Al 2 O 3 composite that was derived from the coked Ni/Al 2 O 3 catalyst. The solutions containing Pb(II), Cr(VI), RhB and MO were separately prepared by dissolving the corresponding nitrates or powders in deionized water. The adsorption experiments were conducted in a 100 mL screw-flask, in which a certain amount of C-Ni/Al 2 O 3 composite (0.01 g for the adsorption of heavy metal ions and 0.05 g for the adsorption of dyes) and 50 mL model pollutant solutions were added. After adsorption, the C-Ni/Al 2 O 3 composite was precipitated and filtered using a 0.22 μm filter. The concentrations of residual heavy metal ions and dyes in the solutions were detected using an atomic adsorption spectrometer (FAAS-M6, Thermo, USA) and a UV-vis spectrophotometer (Shimadzu UV-2600, Japan), respectively. All experiments were performed three times and the average values were presented.  Fig. 1. It is found that the surface of the spent Ni(10%)/Al 2 O 3 catalyst is covered by a mass of fluffy carbon fibers, which are relatively short, thick and cross-linked (Fig. 1b)). Similar fibrous carbon was found on the reacted Ni/Al 2 O 3 catalyst surface according to the report of Alvarez et al., where the Ni/Al 2 O 3 catalyst was used for the catalytic reforming of the mixture of sawdust and different plastics. 24 It is worth noting from Fig. 1b) that catalyst particles can be clearly observed at the end of the fibrous carbon, indicating that the carbon fibers might grow through a top-growth mechanism. The deposited carbon on the Ni/Al 2 O 3 catalyst with too high or too low Ni loadings is dominated by amorphous carbon. For example, a large amount of random particles appear on the reacted Ni(5%)/ Al 2 O 3 catalyst surface (Fig. S1c) and d) †), while as the Ni loading on Al 2 O 3 increases to 20%, loose and irregular carbon is produced on the catalyst surface (Fig. S1e) and f) †) due to the aggregation of catalyst particles with more highly active component in the Ni/Al 2 O 3 catalyst. Fig. 2 depicts the XRD patterns of the fresh catalysts and reacted catalysts with different Ni loadings on Al 2 O 3 catalytically reformed at 600°C. As seen in Fig. 2a), typical NiO diffraction peaks at 37.3°, 63.0°and 75.6°(2θ) are present in the XRD diffraction patterns of the fresh Ni/Al 2 O 3 catalysts, corresponding to NiO with (1 1 1), (2 2 0) and (3 1 1) crystal plane, respectively. 25 It is found that the intensity of NiO-related diffraction peaks is increased gradually with the increase of Ni content in the as-prepared catalysts, and the strongest NiO diffraction peaks are found in Ni(20%)/Al 2 O 3 . The average sizes of NiO are calculated to be 5.2, 7.8 and 12.4 nm with 5%, 10% and 20% Ni loadings, respectively, suggesting that the crystal size of NiO is increased with the enhanced Ni loading on Al 2 O 3 .

Results and discussion
As shown in Fig. 2b), metallic Ni and graphite are reflected in the XRD diffraction patterns of the reacted catalysts. It is clearly observed that metallic Ni diffraction peaks at 2θ = 44.5°, 51.8°, and 76.4°are present in the reacted Ni/Al 2 O 3 catalysts and the diffraction peak intensity is increased with the increase of Ni loading from 5% to 20%. It is noticed that the diffraction peaks of graphite are near 26.5°(2θ) in the XRD patterns of the reacted Ni/Al 2 O 3 catalysts with Ni loadings ranging from 5% to 20%, and the peak intensity of graphite in the patterns of the reacted  (Fig. 1). It is possible that the amount of graphitized carbon produced over Ni(5%)/Al 2 O 3 and Ni(20%)/ Al 2 O 3 during the catalytic reforming process was too low to be observed by SEM.
To cumulatively understand the influence of different Ni loadings on the pyrolysis behavior and thermal stability of the C-Ni/Al 2 O 3 -600°C composite, temperature programmed oxidation (TPO) was used to analyse and the plots of TG and DTG are presented in Fig. 3. It can be found that the weight of the C-Ni(0%)/Al 2 O 3 -600°C composite has no evident change during the whole oxidation process. From Fig. 3a), the weight of the C-Ni(5%)/Al 2 O 3 -600°C composite reaches the maximum at around 500°C and then hardly changes with the increased temperature. The oxidation process of the C-Ni/Al 2 O 3 -600°C composites with Ni loadings of 10% and 20% can be divided into two stages: the first stage from 270°C to 502°C with a weight increment is ascribed to the oxidation of elemental Ni, and the second stage from 502°C to 665°C shows a significant weight loss due to the oxidative decomposition of carbon. The weight loss of the C-Ni(10%)/ Al 2 O 3 -600°C composite as 5.41% is more than that of the C-Ni(20%)/Al 2 O 3 -600°C composite as 2.54%, confirming that a large amount of carbon was deposited on Ni(10%)/Al 2 O 3 during the catalytic reforming process. The influence of Ni loading on the functional groups of the C-Ni/Al 2 O 3 -600°C composite is identified through FTIR analysis, as shown in Fig. 4. The absorbance of the peak at 700-630 cm −1 corresponding to the Al-O stretching vibration is related to the Al 2 O 3 support. The absorption peak at 1110-1044 cm −1 is assigned to the C-O-C stretching vibration 26 and the peak became stronger with the increase of Ni loading, which indicates that the presence of metallic Ni might facilitate the capture of oxygen-containing functional groups from the pyrolysis volatiles of lignin during the catalytic reforming process. The absorption at 1500 cm −1 attributed to the vibration of CC is derived from the aromatic structure of the deposited carbon. 27 At a higher Ni loading, the absorption of -CCC-(2000-1940 cm −1 ) and

View Article Online
-CCO (2150 cm −1 ) was detected, which is probably derived from the intermediates produced from the catalytic reforming of pyrolysis volatiles. The intermediates containing functionalities like -CCCmight be the precursors for carbon formation. 25 In addition, a stretching signal corresponding to -OH functional groups appeared at 3200 cm −1 in the FTIR spectra 28 S2a) and b) †). It is indicated that the active component in the catalyst at lower catalytic reforming temperature could not reform the volatiles from the copyrolysis of lignin and polyethylene and guide the growth of graphitized carbon sufficiently. 9 However, when the catalytic reforming temperature was increased to 800°C, a large number of agglomerated, loose particles are present on the surface of the reacted catalyst (Fig. S2c) and d) †) due to the agglomeration and fusion of the generated carbon. Therefore, it is proposed that a suitable catalytic reforming temperature, i.e., 600-700°C, is required to facilitate the catalytic decomposition of carbon sources and the growth of the graphitized carbon.
XRD patterns of the C-Ni(10%)/Al 2 O 3 composite derived from different catalytic reforming temperatures are shown in Fig. 6. It can be seen that metallic Ni diffraction peaks appeared at 2θ of 44.5°, 51.8°, and 76.4°in all the C-Ni(10%)/Al 2 O 3 composites. It is suggested that the reduction of NiO in the catalyst took place before 500°C. A diffraction peak of graphite at around 26.5°(2θ) was detected in the XRD patterns of the C-Ni(10%)/Al 2 O 3 composites obtained at 600°C and 700°C, but it is absent in those at 500°C and 800°C. This indicated that the production of the graphitized carbon could be around specific temperatures during the catalytic forming process, influencing their performance in the removal of pollutants from wastewater. It is noted that the intensity of the graphite diffraction peak in the XRD pattern of the C-Ni(10%)/Al 2 O 3 composite formed at 700°C was much stronger than that at 600°C, suggesting that more graphitized carbon was produced over Ni(10%)/Al 2 O 3 at the catalytic reforming temperature of 700°C.
The graphitization degree of the deposited carbon on the Ni(10%)/Al 2 O 3 surface is also characterized by Raman spectroscopy, as depicted in Fig. S3. † Three characteristic peaks at around 1332 cm −1 (D band), 1589 cm −1 (G band), and 2770 cm −1 (2D band) were observed, corresponding to the disordered structure or defects in graphene, the sp 2 C-C   Fig. 6. Fig. 7 shows the TPO plots of the C-Ni(10%)/Al 2 O 3 composites derived at different catalytic reforming temperatures from 500 to 800°C. It is found that the weight of the C-Ni(10%)/Al 2 O 3 composites derived at 600, 700 and 800°C are all firstly increased and then decreased, while the weight of the C-Ni(10%)/Al 2 O 3 composite obtained at 500°C is firstly decreased and then increased. The weight increment of the C-Ni(10%)/Al 2 O 3 composites obtained at higher catalytic reforming temperatures is ascribed to the oxidation of metallic Ni in the composite, and the subsequent weight decrease is attributed to the oxidative decomposition of deposited carbon in the composite. The TPO temperature corresponding to the carbon decomposition for the C-Ni(10%)/Al 2 O 3 composite is from 507°C to 710°C, while    Fig. 8 depicts the FTIR spectra of the C-Ni(10%)/Al 2 O 3 composites prepared at different catalytic reforming temperatures (500, 600, 700, 800°C). It can be found that the bands at 3200 cm −1 and 1110-1044 cm −1 correspond to the stretching vibration peaks of OH groups and C-O-C groups, respectively. These vibration peaks appear in the FTIR spectra for all the C-Ni(10%)/Al 2 O 3 composites, and the change of catalytic reforming temperature shows no obvious influence on the peak intensity of oxygen-containing functional groups of the obtained C-Ni(10%)/Al 2 O 3 composites. The absorption bands at around 1500 cm −1 representing the stretching aromatic skeleton vibrations (CC) are observed in all the FTIR spectra of the C-Ni(10%)/Al 2 O 3 composites and the peak intensity becomes stronger with an increase of catalytic reforming temperature, indicating that the increase of catalytic reforming temperature is conducive to the formation of deposited carbon. The absorptions of -CCC-(2000-1940 cm −1 ) and -CCO (2150 cm −1 ) are absent in the FTIR spectra of the C-Ni(10%)/Al 2 O 3 composite derived at 500°C, which is probably attributed to the lack of the intermediates produced from the catalytic reforming of pyrolysis volatiles at a lower temperature.
The N 2 adsorption-desorption isotherms and pore size distribution of the four C-Ni(10%)/Al 2 O 3 composites obtained at the catalytic reforming temperatures from 500°C to 800°C are illustrated in Fig. S4. † It can be found from Fig. S4a) †   Comparing the adsorption performance of the C-Ni/Al 2 O 3 -600°C composites prepared with different Ni loadings, it is found that the removal percentages for Pb(II), Cr(VI), RhB and MO are all dramatically improved with the Ni loading increased from 0 to 10 and then decreased with the Ni loading on Al 2 O 3 increased to 20%. For both heavy metal ions and dyes, the maximum removal percentage is achieved in the case of using the C-Ni(10%)/Al 2 O 3 -600°C composite, suggesting that graphitized carbon with abundant oxygencontaining functional groups has a better adsorption property for the removal of pollutants from wastewater. 30,31 However, increasing the catalytic reforming temperature shows different influences on the removal of the four pollutants from aqueous solution. The maximum adsorption of Pb(II) and RhB is achieved at 700°C with the removal percentage of 88.14% and 72.75%, respectively, while the highest removal percentage for Cr(VI) and MO was 52.42% and 67.99% at 600°C, respectively. The adsorption of Pb(II) was stronger than that of Cr(VI) and the removal percentage for RhB was always higher than that for MO by using all the C-Ni(10%)/Al 2 O 3 composites regardless of the catalytic reforming temperature. Thus, it is concluded that the C-Ni(10%)/Al 2 O 3 -700°C composite was the best adsorbent for the removal of Pb(II) and RhB, while the C-Ni(10%)/Al 2 O 3 -600°C composite was the optimal for the adsorption of Cr(VI) and MO.   3.2.1 Adsorption isotherms. The adsorption isotherms of the heavy metal ions and dyes on the corresponding C-Ni/ Al 2 O 3 composite were investigated by the Langmuir model (eqn (S1) †) and Freundlich model (eqn (S2) †). The isothermal fitting curves are shown in Fig. 10 and the calculated parameters are provided in Table 1. It can be found that the uptakes of the four pollutants using the C-Ni/Al 2 O 3 composite as the adsorbent rapidly increased with the increase of initial concentration until adsorption equilibrium was reached, which can be ascribed to the increase of initial concentration in the initial stage providing higher driving force to overcome the mass transfer resistance of pollutants in solution, 32 and the surface active sites of the C-Ni/Al 2 O 3 composite were completely consumed in the higher range of initial concentration. 33 The Langmuir model was better fitted to the isotherms of the C-Ni/Al 2 O 3 composite with the higher values (0.941-0.979) of the correlation coefficient (R 2 ) obtained from the Langmuir model compared to the Freundlich model. Similar observations were reported in the published studies. [34][35][36] However, according to the study of Abukhadra et al., 37 Fig. 11, and the related kinetic parameters are listed in Table 2. It can be found in Table 2 that the coefficient values (R 2 ) of the pseudo-first-order model are 0.995 and 0.993 for Pb(II) and Cr(VI), respectively, which are higher than those of the pseudo-second-order model (0.961 and 0.991, respectively). Furthermore, the calculated equilibrium adsorption capacity (Q e ) for Pb(II) and Cr(VI) based on the pseudo-first-order model is much closer to the corresponding experimental values (Q exp ). It is suggested that the pseudo-first-order model was more appropriate than the pseudo-second-order model to describe the adsorption processes of Pb(II) and Cr(VI). However, the adsorption processes of RhB and MO are better described by the pseudo-second-order model with R 2 of 0.983-0.988 compared to the pseudo-first-order model (0.912-0.975), suggesting that the pseudo-second-order model is the ideal kinetic model to fit the adsorption processes of RhB and MO. According to the above analysis, it is proposed that reversible reactions frequently takes place in the adsorption processes of heavy metal ions (Pb(II) & Cr(VI)), while the adsorption of dyes (RhB & MO) is dominated by chemical reactions.

Conclusions
In this work, C-Ni/Al 2 O 3 composites derived from the catalytic reforming of volatiles from co-pyrolysis of lignin and polyethylene are used as green adsorbents for the removal of heavy metal ions (Pb(II) & Cr(VI)) and dyes (RhB & MO) from aqueous solutions. The results show that the composition, morphological structure and thermal stability of the carbon deposited on Ni/Al 2 O 3 is significantly influenced by Ni loading in Ni/Al 2 O 3 and the catalytic reforming temperature. In addition, the capture of oxygen-containing functional groups can be enhanced by the higher Ni loading and catalytic reforming temperature, promoting the adsorption of heavy metal ions and dyes. Furthermore, the C-Ni(10%)/ Al 2 O 3 composites obtained at the catalytic reforming temperatures of 600 and 700°C are estimated as the optimal adsorbents for the adsorption of Pb(II), Cr(VI), RhB and MO from aqueous systems. The results show that the adsorption of the C-Ni/Al 2 O 3 composites is dominated by homogeneous monolayer adsorption better fitted by the Langmuir model.

View Article Online
The relationship between the equilibrium adsorption capacity of heavy metal ions and contact time can be well described by the pseudo-first-order kinetic model, while the pseudosecond-order kinetic model gives better fitting for the adsorption of dyes. Therefore, the C-Ni/Al 2 O 3 composite is considered as an environment-friendly and highly efficient adsorbent for treating wastewater containing heavy metal ions and dyes.

Conflicts of interest
There are no conflicts to declare.